Download presentation

Presentation is loading. Please wait.

1
EE130/230A Discussion 2 Peng Zheng

2
**Electron and Hole Concentrations**

Silicon doped with 1016 cm-3 phosphorus atoms, at room temperature (T = 300 K). n = ND = 1016 cm-3, p = 1020/1016 = 104 cm-3 Silicon doped with 1016 cm-3 phosphorus atoms and 1018 cm-3 boron atoms, at room temperature. p = NA - ND = 1018 cm-3, n = 1020/1018 = 102 cm-3 For a compensated semiconductor, i.e. one that has dopants of both types, it is the NET dopant concentration that determines the concentration of the majority carrier. Use np = ni2 to calculate concentration of the minority carrier.

3
**Electron and Hole Concentrations**

Silicon doped with 1016 cm-3 phosphorus atoms and 1018 cm-3 boron atoms, at T = 1000 K NA = 1018 cm-3, ND = 1016 cm-3 ni = 1018 cm-3 at T = 1000 K If ni is comparable to the net dopant concentration. Then the equations on Slide 17 of Lecture 2 must be used to calculate the carrier concentrations accurately. Note, np = ni2 is true at thermal equilibrium.

4
n(Nc, Ec) and p(Nv, Ev)

5
n(ni, Ei) and p(ni, Ei) In an intrinsic semiconductor, n = p = ni and EF = Ei

6
**Carrier distributions**

n-type Material R. F. Pierret, Semiconductor Device Fundamentals, Figure 2.16 Energy band diagram Density of States Probability of occupancy Carrier distributions EE130/230A Fall 2013 Lecture 3, Slide 6

7
**Carrier distributions**

p-type Material R. F. Pierret, Semiconductor Device Fundamentals, Figure 2.16 Energy band diagram Density of States Probability of occupancy Carrier distributions EE130/230A Fall 2013 Lecture 3, Slide 7

8
Fermi level applets

9
Energy band diagram Consider a Si sample maintained under equilibrium conditions, doped with Phosphorus to a concentration 1017 cm-3. For T = 300K, indicate the values of (Ec – EF) and (EF – Ei) in the energy band diagram. Since ni = 1010 cm-3 and n = ni e(EF-Ei)/kT : EF – Ei = kT(ln107) = 7 ∙ kT(ln10) = 7 ∙ 60 meV = 0.42 eV The intrinsic Fermi level is located slightly below midgap: Ec – Ei = Ec – [(Ec+Ev)/2 + (kT/2)∙ln(Nv/Nc)] = (Ec – Ev)/2 – (kT/2)∙ln(Nv/Nc) = 0.56 eV eV = eV Hence Ec – EF = (Ec – Ei) – (EF – Ei) = – 0.42 = eV

10
Energy band diagram For T = 1200K, indicate the values of (Ec – EF) and (EF – Ei). Remember that Nc and Nv are temperature dependent. Also, EG is dependent on temperature: for silicon, EG = 2.8×10-4(T) for T > 300K. At T = 1200K, the Si band gap EG = 1.2 2.8×10-4 (T) = 0.87 eV The conduction-band and valence-band effective densities of states Nc and Nv each have T3/2 dependence, so their product has T3 dependence. (The ratio Nv/Nc does not change with temperature, assuming that the carrier effective masses are independent of temperature.) Therefore, when the temperature is increased by a factor of 4 (from 300K to 1200K), NcNv is increased by a factor of 64. Intrinsic Semiconductor: EF = Ei

Similar presentations

OK

Carrier Concentration in Equilibrium. Since current (electron and hole flow) is dependent on the concentration of electrons and holes in the material,

Carrier Concentration in Equilibrium. Since current (electron and hole flow) is dependent on the concentration of electrons and holes in the material,

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on median and altitude of a triangle Ppt on different occupations workers Ppt on eia report crude Ppt on endangered species in india Ppt on determinants of economic development Raster scan display and random scan display ppt online Ppt on business etiquettes training courses Ppt on 3 idiots movie last part Ppt on strategic management process Ppt on child labour act 1986